Crystal-structure simulation of molecular semiconductors: brickwork-related crystal structures of methylthiolated <i>peri</i>-condensed polycyclic aromatic hydrocarbons.
Bulgarevich, Kirill; Takimiya, Kazuo; Materials horizons 10 (2023) 5492–5499; doi:10.1039/d3mh01055d

data_1570244
_publ_section_title
;
 Crystal-structure simulation of molecular semiconductors:
 brickwork-related crystal structures of methylthiolated
 <i>peri</i>-condensed polycyclic aromatic hydrocarbons.
;
_journal_issue                   12
_journal_name_full               'Materials horizons'
_journal_page_first              5492
_journal_page_last               5499
_journal_paper_doi               10.1039/d3mh01055d
_journal_volume                  10
_journal_year                    2023
_chemical_formula_moiety         'C10 H9 S2'
_chemical_formula_sum            'C10 H9 S2'
_chemical_formula_weight         193.29
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_audit_creation_date             2022-04-13
_audit_creation_method
;
Olex2 1.3-ac4
(compiled 2020.11.27 svn.r5f609507 for Rigaku Oxford Diffraction, GUI svn.r6214)
;
_audit_update_record
;
2023-04-15 deposited with the CCDC.	2023-11-03 downloaded from the CCDC.
;
_cell_angle_alpha                80.578(7)
_cell_angle_beta                 72.733(6)
_cell_angle_gamma                81.783(7)
_cell_formula_units_Z            2
_cell_length_a                   6.5057(5)
_cell_length_b                   7.9795(8)
_cell_length_c                   8.8895(5)
_cell_measurement_reflns_used    2748
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      74.0940
_cell_measurement_theta_min      5.2140
_cell_volume                     432.55(6)
_computing_cell_refinement       'CrysAlisPro 1.171.41.119a (Rigaku OD, 2021)'
_computing_data_collection       'CrysAlisPro 1.171.41.119a (Rigaku OD, 2021)'
_computing_data_reduction        'CrysAlisPro 1.171.41.119a (Rigaku OD, 2021)'
_computing_molecular_graphics    'Olex2 1.3-ac4 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3-ac4 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT  (Sheldrick, 2015)'
_diffrn_ambient_temperature      200(2)
_diffrn_detector                 'Rigaku HyPix-6000 area detector'
_diffrn_detector_area_resol_mean 10.0
_diffrn_detector_type            'HPC area detector'
_diffrn_measured_fraction_theta_full 0.977
_diffrn_measured_fraction_theta_max 0.921
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  t~exp~   \w     \q     \k     \f   Frames
  1  \w    -86.00 -50.00   0.50    8.00    --  -48.00 124.00-140.00   72
  2  \w   -118.00 -93.00   0.50    8.00    --  -48.00-146.00 -25.00   50
  3  \w     66.00  92.00   0.50    8.00    --   48.00-146.00 -25.00   52
  4  \w     33.00  93.00   0.50    8.00    --   48.00-124.00 140.00  120
  5  \w     66.00 107.00   0.50    8.00    --   48.00 146.00  24.00   82
  6  \w   -118.00 -93.00   0.50   20.00    --  -97.00-146.00 -25.00   50
  7  \w   -108.00 -51.00   0.50   20.00    --  -97.00 124.00-140.00  114
  8  \w   -104.00 -78.00   0.50   20.00    --  -97.00 146.00  24.00   52
  9  \w   -126.00-101.00   0.50   20.00    --  -97.00-124.00 140.00   50
 10  \w     34.00  75.00   0.50   20.00    --  104.94-124.00 140.00   82
 11  \w    115.00 140.00   0.50   20.00    --  104.94 124.00-140.00   50
 12  \w     68.00 127.00   0.50   20.00    --  104.94-146.00 -25.00  118
 13  \w     91.00 116.00   0.50   20.00    --  104.94 146.00  24.00   50
 14  \w     82.00 110.00   0.50   20.00    --  104.94-124.00 140.00   56
 15  \w    -71.00 -45.00   0.50    8.00    --  -48.00 146.00  24.00   52
 16  \w    -21.00  22.00   0.50    8.00    --  -48.00  19.00 120.00   86
 17  \w    -20.00   6.00   0.50    8.00    --  -48.00  19.00 -90.00   52
 18  \w     27.00 119.00   0.50    8.00    --   48.00  77.00  30.00  184
 19  \w    -22.00  25.00   0.50    8.00    --   48.00 -19.00-120.00   94
 20  \w    -13.00  25.00   0.50    8.00    --   48.00 -19.00 -90.00   76
 21  \w   -165.00 -89.00   0.50   20.00    --  -97.00 -37.00 -90.00  152
 22  \w   -105.00 -55.00   0.50   20.00    --  -97.00  77.00  30.00  100
 23  \w    -54.00 -25.00   0.50   20.00    --  -97.00  77.00 -30.00   58
 24  \w   -167.00 -90.00   0.50   20.00    --  -97.00 -37.00 120.00  154
 25  \w   -170.00 -90.00   0.50   20.00    --  -97.00 -19.00-180.00  160
 26  \w   -110.00 -84.00   0.50   20.00    --  -97.00 -57.00-150.00   52
 27  \w   -169.00-130.00   0.50   20.00    --  -97.00 -57.00-150.00   78
 28  \w    -91.00 -60.00   0.50   20.00    --  -97.00  77.00 -30.00   62
 29  \w     54.00  79.00   0.50   20.00    --  104.94 -99.00   0.00   50
 30  \w     98.00 162.00   0.50   20.00    --  104.94  37.00  30.00  128
 31  \w     34.00  63.00   0.50   20.00    --  104.94 -57.00-150.00   58
 32  \w     37.00  65.00   0.50   20.00    --  104.94 -57.00  30.00   56
 33  \w     37.00  62.00   0.50   20.00    --  104.94 -57.00 -60.00   50
 34  \w     92.00 172.00   0.50   20.00    --  104.94  57.00 -60.00  160
 35  \w     35.00  63.00   0.50   20.00    --  104.94 -57.00 150.00   56
 36  \w     58.00 106.00   0.50   20.00    --  104.94 -99.00 150.00   96
 37  \w     40.00  65.00   0.50   20.00    --  104.94 -57.00-180.00   50
 38  \w     36.00  61.00   0.50   20.00    --  104.94 -57.00  90.00   50
 39  \w     34.00  81.00   0.50   20.00    --  104.94 -77.00 150.00   94
 40  \w     76.00 106.00   0.50   20.00    --  104.94 -99.00  30.00   60
 41  \w     41.00  66.00   0.50   20.00    --  104.94 -57.00   0.00   50
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Rigaku XtaLAB Synergy-Custom'
_diffrn_measurement_method       '\w scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      0.0337540000
_diffrn_orient_matrix_UB_12      -0.1964565000
_diffrn_orient_matrix_UB_13      0.0156553000
_diffrn_orient_matrix_UB_21      0.2002294000
_diffrn_orient_matrix_UB_22      0.0017311000
_diffrn_orient_matrix_UB_23      0.0582645000
_diffrn_orient_matrix_UB_31      -0.1445130000
_diffrn_orient_matrix_UB_32      -0.0095178000
_diffrn_orient_matrix_UB_33      0.1727620000
_diffrn_radiation_monochromator  'multi-layer mirror optics'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0600
_diffrn_reflns_av_unetI/netI     0.0537
_diffrn_reflns_Laue_measured_fraction_full 0.977
_diffrn_reflns_Laue_measured_fraction_max 0.921
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            4956
_diffrn_reflns_point_group_measured_fraction_full 0.977
_diffrn_reflns_point_group_measured_fraction_max 0.921
_diffrn_reflns_theta_full        67.684
_diffrn_reflns_theta_max         77.531
_diffrn_reflns_theta_min         5.254
_diffrn_source                   'rotating anode X-ray generator'
_diffrn_source_type              micromax007
_exptl_absorpt_coefficient_mu    5.014
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.81299
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.41.119a (Rigaku Oxford Diffraction, 2021)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'clear light yellow'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    yellow
_exptl_crystal_density_diffrn    1.484
_exptl_crystal_description       plate
_exptl_crystal_F_000             202
_exptl_crystal_size_max          0.4
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.001
_refine_diff_density_max         0.790
_refine_diff_density_min         -0.467
_refine_diff_density_rms         0.119
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.161
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     111
_refine_ls_number_reflns         1688
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.161
_refine_ls_R_factor_all          0.0991
_refine_ls_R_factor_gt           0.0875
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1076P)^2^+2.1712P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2609
_refine_ls_wR_factor_ref         0.2665
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1367
_reflns_number_total             1688
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d3mh01055d2.cif
_cod_data_source_block           mt-pyrene_new_plate_200k_220208_autored
_cod_depositor_comments
'Adding full bibliography for 1570243--1570246.cif.'
_cod_database_code               1570244
_shelx_shelxl_version_number     2018/3
_chemical_oxdiff_formula         'C H S'
_shelx_estimated_absorpt_t_max   0.995
_shelx_estimated_absorpt_t_min   0.239
_reflns_odcompleteness_completeness 99.10
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     66.97
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
 At 1.5 times of:
  All C(H,H,H) groups
2.a Aromatic/amide H refined with riding coordinates:
 C10(H10), C6(H6), C4(H4)
2.b Idealised Me refined as rotating group:
 C12(H12A,H12B,H12C), C9(H9A,H9B,H9C)
;
_shelx_res_checksum              65303
_shelx_hkl_checksum              65734
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 3.097
_oxdiff_exptl_absorpt_empirical_full_min 0.469